Transcript of "International Journal of Engineering Inventions (IJEI)"
International Journal of Engineering InventionsISSN: 2278-7461, www.ijeijournal.comVolume 1, Issue 6 (October2012) PP: 01-05 Analysis of Casting Defects and Identification of Remedial Measures – A Diagnostic Study Dr D.N. Shivappa1, Mr Rohit2, Mr. Abhijit Bhattacharya31 Professor, Mechanical Engineering Department, Sir MV Institute of Technology, Bangalore Karnataka India. 2 M Tech Student, Mechanical Engineering Department, Sir MV Institute of Technology, Bangalore India 3 Head Operations, Dakshin Foundry Pvt. Ltd, Bangalore Karnataka India.Abstract––Paper presents analysis of casting defects and identification of remedial measures carried out at DakshinFoundry Ltd, Bangalore, India. Diagnostic study carried out on Trunion Support Bracket (TSB) Castings revealed thatthe contribution of the four prominent defects in casting rejections are sand drop, blow hole, mismatch, and oversize. Itwas noticed that these defects are frequently occurring at particular locations. Systematic analyses were carried out tounderstand the reasons for defects occurrence and suitable remedial measures were identified. Outcome of the validationtrials showed substantial reduction in rejection of castings. Company has accepted the remedial measures andincorporated them in the standard operating procedure. I. INTRODUCTION Dakshin Foundry is facing casting rejections due to some chronic defects, after observing six months’ data of thecompany the most frequently rejected castings identified were TSB, Converter Housing, and Gear Housing. Out of thesethree castings TSB casting was identified as most severely affected casting, hence it was considered for detail investigation.The work on Quality Improvement of castings was carried out in following steps. Identification of defects in the TSB casting and analysis Selection of most chronic defects which frequently occurred and carried out the analysis. Identification of root causes and finding the remedial measures. Production trials in the company with the remedial measures and validation. II. IDENTIFICATION OF CASTING DEFECTS AND ANALYSIS The frequently rejected castings identified at Dakshin Foundry are Trunion Support Bracket (TSB), ConverterHousing, Gear Housing etc. TSB casting comprises 15-20 percent of total production of the company. The number ofcastings produced in the month of June 2010 and their weight, quantity and cost per kg are given in Table 1. As theproduction of TSB is maximum and its cost of rejection is highest this casting was considered for detail study. TSB casting ishaving defects such as sand drop, blow hole, shrinkage, mismatch, sand fusion, core shift, parting line leak, oversize, flash,mould not filled, cold shut etc. The data observation of defects in TSB for six months period from June 2010 to Dec 2010 isplotted as Pareto Chart shown in Figure 1. It may be noticed that the most occurring casting defects are Sand drop, Blowholes, Mismatch, and Oversize hence they were picked up for diagnostic study. To understand the reason for causes of thesefour defects a detail study was carried out in foundry. III. PRODUCTION PROCESS OF TSB CASTING Photograph of the TSB casting is shown in Figure 2. Details of sand systems used for mould and core making areexplained hereunder , .Sand System used for Mould making:Sand: Silica sand 98.5 %Binder: Urea Furan Resin 1% of sandCatalyst: 0.5% of resinSilica sand comprises 85% reclaimed sand and 15% new sand with AFS number 45 to 55, clay content 0.27% (max), andmoisture 0.5% (max). Mixing of sand and binder along with catalyst is done in 20 tonne mixer for 3 to 4 minutes.Sand System used for Core making:Four cores are used in TSB casting, these are central core, breaker core, U cut core, flat core.Sand system used for central core, U cut core, breaker core are;Sand: Silica sand 98.5 %Binder: Urea Furan Resin 1% of sandCatalyst: 0.5% of resinSand system used for flat core are;Sand: Silica sand 96.5 %Binder: Sodium silicate 3.5 % 1
Analysis of Casting Defects and Identification of Remedial Measures... For all the cores fresh silica sand is used, in case of resin bonded core the sand system is prepared as explainedabove for moulding sand system. And for sodium silicate – Co2 sand system mixing of fresh silica sand and sodium silica isdone in mixer for 3 minutes. Soon after the mixing core sand mix is taken to core box and adequately rammed, after theramming Co2 gas is passed into core box for 60 seconds. After the moulds and cores are cured, and securing them properlythe molten metal is poured and allowed to solidify. After 8 hours of pouring shakeout of casting is done and processedfurther. Inspection of casting is done at different stages as per the requirement .Chemical constituents of TSB casting are: Fe 92-94%, C 3.20-3.60%, Si 2.20-2.60%, Mn 0.60%, P 0.05%, S0.015%, Mg0.025-0.050%, etc. IV. CASTING DEFECTS ANALYSIS AND REMEDIAL MEASURES Analysis for causes of most frequently occurring four defects of TSB casting are carried out. The reason foroccurrence of these defects and their remedial measure are briefly given in Table 2. Due to nature of defects they wereanalysed by observation in the shop-floor for quite a long period and assessed. Wisdom of the experts in the company andlong experience of the authors in the field of foundry technology has helped in identifying the nature of causes. Repeatedtrials were carried out in the foundry to arrive at appropriate remedial measures. V. VALIDATION WITH PRODUCTION TRIALS Production trials on TSB casting were carried out in the company after incorporating the remedial measuresidentified and reported in section 4 above. There is a substantial improvement in quality resulting in reduction in rejectionlevels of castings, details are given in Table 3. For the purpose of comparison four months data of TSB Casting beforeimplementation of remedial is compared with four months data after implementation of remedial measure, details ofvalidation trials are presented here below. And it is noted that number of TSB castings produced during these four monthsperiod are; 2657 and 2730 respectively of the years 2010 and 2011. Since difference in production quantity is only about2.7% it is considered as same for the purpose of comparisons of rejection quantity before and after implementation ofremedial measure.(i) Remedial measure trial for sand drop defect As reported Table 2 loose sand at chill and moulds interface left un-cleaned at long member that was resulting insand drop in this location. This was happening due to carelessness of operators. Strict instructions were given to theoperators for ensuring the proper cleaning of moulds before closing and not cleaning the mould when two moulds are near.That suggestion is also revised in mould making checklist. By proper monitoring of cleaning moulds before closing, it wasobserved that before remedial measure 52 castings were rejected due to sand drop found around long member but afterimplementation of remedial measure only 18 castings were rejected during four months period. The reduction in castingsrejection was observed as 65.4%.The second reason for rejection of TSB casting due to sand drop found around square pad area. Due to sleeve top hole, thesand enters through sleeves and gets collected around the bottom of surface of top and bottom pad. Here also impropercleaning of sleeve hole was reason for rejection due to sand drop. The remedial measure taken was to cover the sleeve tophole by paper and clean the hole by air blowing and remove the paper before pouring. After implementation of this smallcorrection, castings rejection reduced by 75.6%, details are given in Table 3.Core oversize and core end broken were also found responsible for rejections of TSB casting, due to these reason sand dropobserved around cross member. To overcome the problem loose piece design modified in core box, and also two pads wereprovided at the bottom face of core. The remedial measure implemented and observed the rejections data for last four monthwhich showed 84.6% reduction in rejections.(ii) Remedial measure trial for blow-hole defect To overcome the TSB casting rejections due to blow holes observed at chill interface area the position of flow offsin gating design was modified. The placement of flow offs at the right position in gating system was very difficult but aftertaking 3 to 4 trials and observation, it was found that the correct position of flow offs on the top surface of long memberonly. This change brought down the rejection level by 67%.(iii) Remedial measure trial for mismatch defect The inadequate numbers of locators were found to be responsible for mismatch of TSB casting. Initially only threemetallic locators were placed to locate bottom and top mould, but in order to resist mould or core movement some morelocators were required. At the time of trials the mounting of extra number of locators was found difficult. During first trialonly two locators were mounted in diagonally opposite direction, but this concept didn’t show much improvement. Then insecond trial three locators were placed in a triangular manner, the two locators were placed on a single line and thirdopposite side of the line. There are three cavities provided at the pattern and three self sand mould locators build for thecavity. Now the six locators (metallic and self sand) are used to overcome the problem of mismatch. The four monthrejection data shows that before remedial measure the rejections were 43 castings due to mismatch but after remedialmeasures only 7 castings rejected, which show 83.7% improvement in mismatch.(iv) Remedial measure trial for oversize problem 2
Analysis of Casting Defects and Identification of Remedial Measures... Oversize of casting was another reasons for rejection of TSB casting. Due to mould bulging and mould liftoversize of castings used to take place. This was happening due to improper clamping of moulds. Initially in the first trialonly c- channel clamp was provided at sideways. But it was found that this measure was not suitable to control mouldbulging at centre. Then in the second trial along with sideways channels an intermediate c- channel clamp was provided.This measure reduced the casting rejection by 77%.After confirming with four months results by adopting remedial measures and noticing the substantial quality improvement,company accepted the measures suggested in the work. Standard operating procedures of the company were revised byincorporating the suggested measures. VI. CONCLUSION Diagnostic study carried out on TSB Castings revealed that the contribution of the four prominent defects incasting rejections are Sand drop, Blow hole, Mismatch, and Oversize. It was noticed that these defects are frequentlyoccurring at particular locations. Systematic analyses were carried out to understand the reasons for defects occurrence andthe reasons identified are; The causes of sand drop were found due to improper cleaning of mould in the areas around chills and mould interface, sleeve, and breaker core. Blow holes occurrence around long member is due to failure to connect flow off in the gating design. The mismatch of castings is due to lack of locators and improper setting of cores. Casting oversize is due to mould lift and mould bulging.Remedial measures identified to overcome the above defects are; (i) Sand Drop: Proper cleaning of the mould before closing, ensure that sand don’t enter into the sleeve, replace no- bake core with shell core, provide pads at bottom face, and modified the loose piece design to avoid core crushing. (i) Blow Hole: Modification of gating system; flow offs are to be directly connected on top surface of long member. (ii) Mismatch: Provided six locators for proper setting of cores - three are of metallic and three are self locators. (iii) Oversize: Clamp the moulds properly to withstand the pouring pressure – Clamp centre channel with C-Clamps during metal pouring.Production trials were carried out in the foundry for four months period by incorporating the above remedial measures andvalidated. Outcome of the results showed substantial reduction in rejection of castings. Company has accepted and adoptedthe remedial measures suggested in the production methods, also suitably modified the standard operating procedure. REFERENCES 1. British Cast Iron Research Association, ‘BCIRA broadsheets’, BCIRA, 1986. 2. Apex Company (Dhakshin Foundry) Manual. 3. American Foundry Men’s Society, ‘Analysis of casting defects’, American Foundry Men’s Society, USA, 1974.Acknowledgement: Authors sincerely express their gratitude to the Management and Employees of Dakshin Foundry Ltd,Bangalore, India for their help, support, and assistance. Weight Rejection Cost (Rs) per Cost of Rejection, Casting (Kg) Produc-tion Quantity Kg Rs Name Quantity (A) (B) (C ) (A×B×C) TSB 83 748 40 99 328,680 Converter 250 70 5 95.5 119,375 Housing Gear 202 23 5 349 96,455 Housing Rs: Indian Rupe Table 1 Details of Rejected Castings in June 2010 3
Analysis of Casting Defects and Identification of Remedial Measures...SI. Remedial Measure Defect Name Defect Location CausesNo. (RM) Before closing the mould, ensure the Chill and mould interface Long member cleaning of mould, chill and mould not cleaned properly interface. Close the sleeve top hole by covering Square pad area: Sleeve inside loose sand not paper before mould closing and remove Top & Bottom 40 cleaned up at the time of pouring. mm area1 Sand Drop Around Breaker Loose sand around the Core breaker core is due to Replace No-Bake core with Shell core improper sand ramming Core crushing while core Loose piece design modified setting. Cross member Core end broken and fallen Two pads provided at the bottom face inside mould Around chill Failure to connect Flow2 Blow Hole Flow off provided on the casting face interface area Offs Lack of locators in pattern Provide six locators three are metallic3 Mismatch Around the Bore and improper setting of and three are self locator cores Improper clamping of Centre clamping with C-clamps4 Oversize moulds, mould lift and mould bulging Table 2 Major Sand Drop Location, Causes & Remedial Measure Rejection* Before Rejection** After SI. Reduction in Defects Defect Location RM RM No. Rejection (percent) (Quantity) (Quantity) Long member 52 18 65.4 1. Sand Drop Square pad area 41 10 75.6 Cross member 26 4 84.6 2. Blow Holes Around chill area 36 12 67.0 3. Mismatch Around bore 43 7 83.7 4. Oversize - 48 11 77.0 RM: Remedial Measure, * During March – June 2010, ** During March – June2011 Table 3 Rejection Control after Remedial Measure 4
Analysis of Casting Defects and Identification of Remedial Measures... 120.0 97.7 100Percentage of Rejection 100.0 89.1 80.1 80.0 58.8 60.0 40.0 32.6 26.2 21.3 20.0 9 8.6 2.3 0.0 Sand drop Blow holes Mismatch Over size Core Lift Shrinkage Defects Percentage Rejection Percentage Cummulative Rejection Figure 1 Pareto Diagram of Defects Figure 2 Photograph of TSB Casting in TSB Casting 5